cometadata/datacite-titles-descriptions-related-identifiers huggingface dataset:
DOI: 10.17188/1268033
title: Materials Data on CaGe2O5 by Materials Project

description: CaGe2O5 is Esseneite-derived structured and crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are two inequivalent Ca2+ sites. In the first Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.30–2.90 Å. In the second Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.30–2.93 Å. There are four inequivalent Ge4+ sites. In the first Ge4+ site, Ge4+ is bonded to four O2- atoms to form corner-sharing GeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 43–57°. There is two shorter (1.77 Å) and two longer (1.78 Å) Ge–O bond length. In the second Ge4+ site, Ge4+ is bonded to six O2- atoms to form GeO6 octahedra that share corners with two equivalent GeO6 octahedra and corners with four GeO4 tetrahedra. The corner-sharing octahedral tilt angles are 40°. There are a spread of Ge–O bond distances ranging from 1.85–2.00 Å. In the third Ge4+ site, Ge4+ is bonded to four O2- atoms to form corner-sharing GeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 43–57°. There is two shorter (1.77 Å) and two longer (1.78 Å) Ge–O bond length. In the fourth Ge4+ site, Ge4+ is bonded to six O2- atoms to form GeO6 octahedra that share corners with two equivalent GeO6 octahedra and corners with four GeO4 tetrahedra. The corner-sharing octahedral tilt angles are 40°. There are a spread of Ge–O bond distances ranging from 1.86–1.98 Å. There are ten inequivalent O2- sites. In the first O2- site, O2- is bonded in a distorted trigonal planar geometry to one Ca2+ and two Ge4+ atoms. In the second O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Ge4+ atoms. In the third O2- site, O2- is bonded in a distorted trigonal planar geometry to one Ca2+ and two Ge4+ atoms. In the fourth O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Ge4+ atoms. In the fifth O2- site, O2- is bonded to two Ca2+ and two Ge4+ atoms to form a mixture of distorted corner and edge-sharing OCa2Ge2 tetrahedra. In the sixth O2- site, O2- is bonded to two Ca2+ and two Ge4+ atoms to form a mixture of distorted corner and edge-sharing OCa2Ge2 tetrahedra. In the seventh O2- site, O2- is bonded in a 3-coordinate geometry to one Ca2+ and two Ge4+ atoms. In the eighth O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Ge4+ atoms. In the ninth O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Ge4+ atoms. In the tenth O2- site, O2- is bonded in a 3-coordinate geometry to one Ca2+ and two Ge4+ atoms.
DOI: 10.17188/1268034
title: Materials Data on ZnS by Materials Project

description: ZnS is Moissanite 9R-like structured and crystallizes in the trigonal P3m1 space group. The structure is three-dimensional. there are five inequivalent Zn2+ sites. In the first Zn2+ site, Zn2+ is bonded to four S2- atoms to form corner-sharing ZnS4 tetrahedra. All Zn–S bond lengths are 2.36 Å. In the second Zn2+ site, Zn2+ is bonded to four S2- atoms to form corner-sharing ZnS4 tetrahedra. All Zn–S bond lengths are 2.36 Å. In the third Zn2+ site, Zn2+ is bonded to four S2- atoms to form corner-sharing ZnS4 tetrahedra. All Zn–S bond lengths are 2.36 Å. In the fourth Zn2+ site, Zn2+ is bonded to four S2- atoms to form corner-sharing ZnS4 tetrahedra. All Zn–S bond lengths are 2.36 Å. In the fifth Zn2+ site, Zn2+ is bonded to four S2- atoms to form corner-sharing ZnS4 tetrahedra. All Zn–S bond lengths are 2.36 Å. There are six inequivalent S2- sites. In the first S2- site, S2- is bonded to four Zn2+ atoms to form corner-sharing SZn4 tetrahedra. In the second S2- site, S2- is bonded to four Zn2+ atoms to form corner-sharing SZn4 tetrahedra. In the third S2- site, S2- is bonded to four equivalent Zn2+ atoms to form corner-sharing SZn4 tetrahedra. In the fourth S2- site, S2- is bonded to four Zn2+ atoms to form corner-sharing SZn4 tetrahedra. All S–Zn bond lengths are 2.36 Å. In the fifth S2- site, S2- is bonded to four Zn2+ atoms to form corner-sharing SZn4 tetrahedra. The S–Zn bond length is 2.36 Å. In the sixth S2- site, S2- is bonded to four Zn2+ atoms to form corner-sharing SZn4 tetrahedra.
DOI: 10.17188/1268036
title: Materials Data on MgAs2(XeF9)2 by Materials Project

description: MgAs2(XeF9)2 crystallizes in the monoclinic P2_1/c space group. The structure is two-dimensional and consists of one MgAs2(XeF9)2 sheet oriented in the (-1, 0, 2) direction. there are two inequivalent Xe sites. In the first Xe site, Xe is bonded in a linear geometry to two F atoms. There are one shorter (2.02 Å) and one longer (2.13 Å) Xe–F bond lengths. In the second Xe site, Xe is bonded in a rectangular see-saw-like geometry to four F atoms. There are a spread of Xe–F bond distances ranging from 1.99–2.15 Å. Mg is bonded to six F atoms to form MgF6 octahedra that share corners with four AsF6 octahedra. The corner-sharing octahedra tilt angles range from 30–38°. There are a spread of Mg–F bond distances ranging from 1.98–2.05 Å. There are two inequivalent As sites. In the first As site, As is bonded to six F atoms to form AsF6 octahedra that share corners with two equivalent MgF6 octahedra. The corner-sharing octahedra tilt angles range from 35–38°. There are a spread of As–F bond distances ranging from 1.75–1.84 Å. In the second As site, As is bonded to six F atoms to form AsF6 octahedra that share corners with two equivalent MgF6 octahedra. The corner-sharing octahedral tilt angles are 30°. There are a spread of As–F bond distances ranging from 1.75–1.84 Å. There are eighteen inequivalent F sites. In the first F site, F is bonded in a single-bond geometry to one As atom. In the second F site, F is bonded in a bent 150 degrees geometry to one Mg and one As atom. In the third F site, F is bonded in a bent 150 degrees geometry to one Mg and one As atom. In the fourth F site, F is bonded in a bent 150 degrees geometry to one Mg and one As atom. In the fifth F site, F is bonded in a single-bond geometry to one As atom. In the sixth F site, F is bonded in a single-bond geometry to one Xe atom. In the seventh F site, F is bonded in a bent 150 degrees geometry to one Xe and one Mg atom. In the eighth F site, F is bonded in a single-bond geometry to one Xe atom. In the ninth F site, F is bonded in a single-bond geometry to one As atom. In the tenth F site, F is bonded in a single-bond geometry to one As atom. In the eleventh F site, F is bonded in a single-bond geometry to one As atom. In the twelfth F site, F is bonded in a single-bond geometry to one Xe atom. In the thirteenth F site, F is bonded in a linear geometry to one Xe and one Mg atom. In the fourteenth F site, F is bonded in a single-bond geometry to one As atom. In the fifteenth F site, F is bonded in a single-bond geometry to one As atom. In the sixteenth F site, F is bonded in a bent 150 degrees geometry to one Mg and one As atom. In the seventeenth F site, F is bonded in a single-bond geometry to one Xe atom. In the eighteenth F site, F is bonded in a single-bond geometry to one As atom.
DOI: 10.17188/1268037
title: Materials Data on Ba6Na2As2Ru2O17 by Materials Project

description: Na2Ba6Ru2As2O17 crystallizes in the hexagonal P6_3/mmc space group. The structure is three-dimensional. Na1+ is bonded to six O2- atoms to form NaO6 octahedra that share corners with three equivalent RuO6 octahedra, corners with three equivalent AsO4 tetrahedra, and a faceface with one BaO12 cuboctahedra. The corner-sharing octahedral tilt angles are 5°. There are three shorter (2.29 Å) and three longer (2.38 Å) Na–O bond lengths. There are four inequivalent Ba2+ sites. In the first Ba2+ site, Ba2+ is bonded in a 10-coordinate geometry to ten O2- atoms. There are a spread of Ba–O bond distances ranging from 2.63–3.03 Å. In the second Ba2+ site, Ba2+ is bonded in a distorted q6 geometry to nine O2- atoms. There are three shorter (2.80 Å) and six longer (2.99 Å) Ba–O bond lengths. In the third Ba2+ site, Ba2+ is bonded in a 12-coordinate geometry to six equivalent O2- atoms. All Ba–O bond lengths are 2.84 Å. In the fourth Ba2+ site, Ba2+ is bonded to twelve O2- atoms to form BaO12 cuboctahedra that share corners with six equivalent BaO12 cuboctahedra, faces with two equivalent NaO6 octahedra, and faces with six equivalent RuO6 octahedra. There are six shorter (2.97 Å) and six longer (3.02 Å) Ba–O bond lengths. Ru5+ is bonded to six O2- atoms to form RuO6 octahedra that share corners with three equivalent NaO6 octahedra, faces with three equivalent BaO12 cuboctahedra, and a faceface with one RuO6 octahedra. The corner-sharing octahedral tilt angles are 5°. There are three shorter (1.90 Å) and three longer (2.10 Å) Ru–O bond lengths. As5+ is bonded to four O2- atoms to form AsO4 tetrahedra that share corners with three equivalent NaO6 octahedra. The corner-sharing octahedral tilt angles are 19°. There is one shorter (1.71 Å) and three longer (1.73 Å) As–O bond length. There are four inequivalent O2- sites. In the first O2- site, O2- is bonded in a 2-coordinate geometry to one Na1+, four Ba2+, and one Ru5+ atom. In the second O2- site, O2- is bonded to four Ba2+ and two equivalent Ru5+ atoms to form a mixture of distorted face and corner-sharing OBa4Ru2 octahedra. The corner-sharing octahedra tilt angles range from 6–60°. In the third O2- site, O2- is bonded in a 5-coordinate geometry to one Na1+, three Ba2+, and one As5+ atom. In the fourth O2- site, O2- is bonded in a distorted linear geometry to one Ba2+ and one As5+ atom.
DOI: 10.17188/1268038
title: Materials Data on Ba6Hf5S16 by Materials Project

description: Ba6Hf5S16 is (Cubic) Perovskite-like structured and crystallizes in the tetragonal I4/mmm space group. The structure is three-dimensional. there are three inequivalent Ba2+ sites. In the first Ba2+ site, Ba2+ is bonded in a 9-coordinate geometry to nine S2- atoms. There are a spread of Ba–S bond distances ranging from 3.13–3.57 Å. In the second Ba2+ site, Ba2+ is bonded to twelve S2- atoms to form BaS12 cuboctahedra that share corners with eight BaS12 cuboctahedra, faces with five BaS12 cuboctahedra, and faces with eight HfS6 octahedra. There are a spread of Ba–S bond distances ranging from 3.46–3.59 Å. In the third Ba2+ site, Ba2+ is bonded to twelve S2- atoms to form BaS12 cuboctahedra that share corners with twelve BaS12 cuboctahedra, faces with six BaS12 cuboctahedra, and faces with eight HfS6 octahedra. There are a spread of Ba–S bond distances ranging from 3.52–3.56 Å. There are three inequivalent Hf4+ sites. In the first Hf4+ site, Hf4+ is bonded to six S2- atoms to form HfS6 octahedra that share corners with six HfS6 octahedra and faces with eight BaS12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–1°. There are a spread of Hf–S bond distances ranging from 2.49–2.53 Å. In the second Hf4+ site, Hf4+ is bonded to six S2- atoms to form HfS6 octahedra that share corners with six HfS6 octahedra and faces with eight equivalent BaS12 cuboctahedra. The corner-sharing octahedral tilt angles are 0°. There are four shorter (2.50 Å) and two longer (2.51 Å) Hf–S bond lengths. In the third Hf4+ site, Hf4+ is bonded to six S2- atoms to form HfS6 octahedra that share corners with five HfS6 octahedra and faces with four equivalent BaS12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–6°. There are a spread of Hf–S bond distances ranging from 2.49–2.59 Å. There are six inequivalent S2- sites. In the first S2- site, S2- is bonded in a distorted linear geometry to four equivalent Ba2+ and two equivalent Hf4+ atoms. In the second S2- site, S2- is bonded in a 6-coordinate geometry to five equivalent Ba2+ and one Hf4+ atom. In the third S2- site, S2- is bonded in a distorted linear geometry to four equivalent Ba2+ and two Hf4+ atoms. In the fourth S2- site, S2- is bonded in a 2-coordinate geometry to four Ba2+ and two equivalent Hf4+ atoms. In the fifth S2- site, S2- is bonded in a distorted linear geometry to four Ba2+ and two equivalent Hf4+ atoms. In the sixth S2- site, S2- is bonded in a distorted linear geometry to four equivalent Ba2+ and two Hf4+ atoms.
DOI: 10.17188/1268039
title: Materials Data on CaCr2O4 (SG:59) by Materials Project

description: Computed materials data using density functional theory calculations. These calculations determine the electronic structure of bulk materials by solving approximations to the Schrodinger equation. For more information, see https://materialsproject.org/docs/calculations
DOI: 10.17188/1268040
title: Materials Data on La2Mo4O15 (SG:14) by Materials Project

description: Computed materials data using density functional theory calculations. These calculations determine the electronic structure of bulk materials by solving approximations to the Schrodinger equation. For more information, see https://materialsproject.org/docs/calculations
DOI: 10.17188/1268041
title: Materials Data on GePbO3 by Materials Project

description: PbGeO3 crystallizes in the trigonal R-3 space group. The structure is three-dimensional. Pb2+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Pb–O bond distances ranging from 2.30–2.60 Å. Ge4+ is bonded to four O2- atoms to form corner-sharing GeO4 tetrahedra. There are a spread of Ge–O bond distances ranging from 1.76–1.80 Å. There are three inequivalent O2- sites. In the first O2- site, O2- is bonded in a bent 120 degrees geometry to two equivalent Ge4+ atoms. In the second O2- site, O2- is bonded in a distorted single-bond geometry to three equivalent Pb2+ and one Ge4+ atom. In the third O2- site, O2- is bonded in a distorted trigonal planar geometry to two equivalent Pb2+ and one Ge4+ atom.
DOI: 10.17188/1268042
title: Materials Data on Mg2B2O5 by Materials Project

description: Mg2B2O5 crystallizes in the triclinic P-1 space group. The structure is three-dimensional. there are two inequivalent Mg2+ sites. In the first Mg2+ site, Mg2+ is bonded to six O2- atoms to form distorted edge-sharing MgO6 octahedra. There are a spread of Mg–O bond distances ranging from 2.00–2.27 Å. In the second Mg2+ site, Mg2+ is bonded to six O2- atoms to form edge-sharing MgO6 octahedra. There are a spread of Mg–O bond distances ranging from 2.04–2.18 Å. There are two inequivalent B3+ sites. In the first B3+ site, B3+ is bonded in a trigonal planar geometry to three O2- atoms. There are a spread of B–O bond distances ranging from 1.35–1.43 Å. In the second B3+ site, B3+ is bonded in a trigonal planar geometry to three O2- atoms. There are a spread of B–O bond distances ranging from 1.36–1.44 Å. There are five inequivalent O2- sites. In the first O2- site, O2- is bonded to three Mg2+ and one B3+ atom to form a mixture of distorted edge and corner-sharing OMg3B trigonal pyramids. In the second O2- site, O2- is bonded in a 4-coordinate geometry to three equivalent Mg2+ and one B3+ atom. In the third O2- site, O2- is bonded in a 3-coordinate geometry to one Mg2+ and two B3+ atoms. In the fourth O2- site, O2- is bonded in a distorted trigonal planar geometry to two equivalent Mg2+ and one B3+ atom. In the fifth O2- site, O2- is bonded to three Mg2+ and one B3+ atom to form a mixture of distorted edge and corner-sharing OMg3B tetrahedra.
DOI: 10.17188/1268043
title: Materials Data on SbP(OF3)2 by Materials Project

description: SbP(OF3)2 crystallizes in the triclinic P-1 space group. The structure is zero-dimensional and consists of one SbP(OF3)2 cluster. Sb5+ is bonded to two O2- and four F1- atoms to form SbO2F4 octahedra that share corners with two equivalent PO2F2 tetrahedra. Both Sb–O bond lengths are 2.06 Å. There is three shorter (1.89 Å) and one longer (1.91 Å) Sb–F bond length. P5+ is bonded to two O2- and two F1- atoms to form PO2F2 tetrahedra that share corners with two equivalent SbO2F4 octahedra. The corner-sharing octahedra tilt angles range from 43–44°. There is one shorter (1.51 Å) and one longer (1.52 Å) P–O bond length. There is one shorter (1.53 Å) and one longer (1.54 Å) P–F bond length. There are two inequivalent O2- sites. In the first O2- site, O2- is bonded in a 2-coordinate geometry to one Sb5+ and one P5+ atom. In the second O2- site, O2- is bonded in a 2-coordinate geometry to one Sb5+ and one P5+ atom. There are six inequivalent F1- sites. In the first F1- site, F1- is bonded in a single-bond geometry to one Sb5+ atom. In the second F1- site, F1- is bonded in a single-bond geometry to one P5+ atom. In the third F1- site, F1- is bonded in a single-bond geometry to one P5+ atom. In the fourth F1- site, F1- is bonded in a single-bond geometry to one Sb5+ atom. In the fifth F1- site, F1- is bonded in a single-bond geometry to one Sb5+ atom. In the sixth F1- site, F1- is bonded in a single-bond geometry to one Sb5+ atom.
DOI: 10.17188/1268044
title: Materials Data on NaZr2NiF11 by Materials Project

description: NaZr2NiF11 crystallizes in the monoclinic C2/m space group. The structure is three-dimensional. Na1+ is bonded to eight F1- atoms to form distorted NaF8 hexagonal bipyramids that share corners with two equivalent ZrF7 pentagonal bipyramids, edges with two equivalent NiF6 octahedra, and edges with four equivalent ZrF7 pentagonal bipyramids. There are four shorter (2.23 Å) and four longer (2.78 Å) Na–F bond lengths. Zr4+ is bonded to seven F1- atoms to form ZrF7 pentagonal bipyramids that share a cornercorner with one NaF8 hexagonal bipyramid, corners with three equivalent NiF6 octahedra, a cornercorner with one ZrF7 pentagonal bipyramid, edges with two equivalent NaF8 hexagonal bipyramids, and an edgeedge with one ZrF7 pentagonal bipyramid. The corner-sharing octahedra tilt angles range from 8–33°. There are a spread of Zr–F bond distances ranging from 1.98–2.18 Å. Ni2+ is bonded to six F1- atoms to form NiF6 octahedra that share corners with six equivalent ZrF7 pentagonal bipyramids and edges with two equivalent NaF8 hexagonal bipyramids. There are two shorter (2.02 Å) and four longer (2.06 Å) Ni–F bond lengths. There are five inequivalent F1- sites. In the first F1- site, F1- is bonded in a distorted bent 150 degrees geometry to one Na1+, one Zr4+, and one Ni2+ atom. In the second F1- site, F1- is bonded in a linear geometry to two equivalent Zr4+ atoms. In the third F1- site, F1- is bonded in a trigonal planar geometry to one Na1+ and two equivalent Zr4+ atoms. In the fourth F1- site, F1- is bonded in a linear geometry to one Zr4+ and one Ni2+ atom. In the fifth F1- site, F1- is bonded in a linear geometry to one Na1+ and one Zr4+ atom.
DOI: 10.17188/1268045
title: Materials Data on TiPHO5 by Materials Project

description: Ti(OH)PO4 crystallizes in the monoclinic P2_1 space group. The structure is three-dimensional. there are two inequivalent Ti4+ sites. In the first Ti4+ site, Ti4+ is bonded to six O2- atoms to form distorted TiO6 octahedra that share corners with two equivalent TiO6 octahedra and corners with four PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 35–49°. There are a spread of Ti–O bond distances ranging from 1.81–2.41 Å. In the second Ti4+ site, Ti4+ is bonded to six O2- atoms to form distorted TiO6 octahedra that share corners with two equivalent TiO6 octahedra and corners with four PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 35–49°. There are a spread of Ti–O bond distances ranging from 1.81–2.41 Å. There are two inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with four TiO6 octahedra. The corner-sharing octahedra tilt angles range from 26–37°. There is one shorter (1.54 Å) and three longer (1.55 Å) P–O bond length. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with four TiO6 octahedra. The corner-sharing octahedra tilt angles range from 39–41°. There is two shorter (1.54 Å) and two longer (1.55 Å) P–O bond length. There are two inequivalent H1+ sites. In the first H1+ site, H1+ is bonded in a single-bond geometry to one O2- atom. The H–O bond length is 0.99 Å. In the second H1+ site, H1+ is bonded in a single-bond geometry to one O2- atom. The H–O bond length is 0.99 Å. There are ten inequivalent O2- sites. In the first O2- site, O2- is bonded in a water-like geometry to two Ti4+ and two H1+ atoms. In the second O2- site, O2- is bonded in a bent 150 degrees geometry to one Ti4+ and one P5+ atom. In the third O2- site, O2- is bonded in a bent 150 degrees geometry to two Ti4+ atoms. In the fourth O2- site, O2- is bonded in a bent 150 degrees geometry to one Ti4+ and one P5+ atom. In the fifth O2- site, O2- is bonded in a bent 150 degrees geometry to one Ti4+ and one P5+ atom. In the sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one Ti4+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a bent 150 degrees geometry to one Ti4+ and one P5+ atom. In the eighth O2- site, O2- is bonded in a bent 150 degrees geometry to one Ti4+ and one P5+ atom. In the ninth O2- site, O2- is bonded in a bent 150 degrees geometry to one Ti4+ and one P5+ atom. In the tenth O2- site, O2- is bonded in a bent 150 degrees geometry to one Ti4+ and one P5+ atom.
DOI: 10.17188/1268046
title: Materials Data on AsSe(ClF2)3 by Materials Project

description: AsSe(ClF2)3 crystallizes in the monoclinic P2_1/c space group. The structure is one-dimensional and consists of two AsSe(ClF2)3 ribbons oriented in the (0, 1, 0) direction. As5+ is bonded in an octahedral geometry to six F1- atoms. There are a spread of As–F bond distances ranging from 1.76–1.80 Å. Se4+ is bonded in a distorted trigonal non-coplanar geometry to three Cl1- atoms. There are two shorter (2.14 Å) and one longer (2.15 Å) Se–Cl bond lengths. There are three inequivalent Cl1- sites. In the first Cl1- site, Cl1- is bonded in a 1-coordinate geometry to one Se4+ and one F1- atom. The Cl–F bond length is 2.94 Å. In the second Cl1- site, Cl1- is bonded in a distorted single-bond geometry to one Se4+ atom. In the third Cl1- site, Cl1- is bonded in a 1-coordinate geometry to one Se4+ and one F1- atom. The Cl–F bond length is 2.96 Å. There are six inequivalent F1- sites. In the first F1- site, F1- is bonded in a single-bond geometry to one As5+ atom. In the second F1- site, F1- is bonded in a single-bond geometry to one As5+ atom. In the third F1- site, F1- is bonded in a single-bond geometry to one As5+ atom. In the fourth F1- site, F1- is bonded in a single-bond geometry to one As5+ and one Cl1- atom. In the fifth F1- site, F1- is bonded in a single-bond geometry to one As5+ and one Cl1- atom. In the sixth F1- site, F1- is bonded in a single-bond geometry to one As5+ atom.
DOI: 10.17188/1268054
title: Materials Data on Cs2Mo15S19 by Materials Project

description: Cs2Mo15S19 crystallizes in the trigonal R-3c space group. The structure is three-dimensional. Cs1+ is bonded in a 11-coordinate geometry to eleven S2- atoms. There are a spread of Cs–S bond distances ranging from 3.31–3.80 Å. There are three inequivalent Mo+2.40+ sites. In the first Mo+2.40+ site, Mo+2.40+ is bonded to five S2- atoms to form a mixture of edge and corner-sharing MoS5 square pyramids. There are a spread of Mo–S bond distances ranging from 2.42–2.65 Å. In the second Mo+2.40+ site, Mo+2.40+ is bonded to five S2- atoms to form a mixture of edge and corner-sharing MoS5 square pyramids. There are a spread of Mo–S bond distances ranging from 2.42–2.47 Å. In the third Mo+2.40+ site, Mo+2.40+ is bonded in a see-saw-like geometry to four S2- atoms. There are two shorter (2.40 Å) and two longer (2.48 Å) Mo–S bond lengths. There are five inequivalent S2- sites. In the first S2- site, S2- is bonded in a 6-coordinate geometry to two equivalent Cs1+ and four Mo+2.40+ atoms. In the second S2- site, S2- is bonded in a 5-coordinate geometry to one Cs1+ and four Mo+2.40+ atoms. In the third S2- site, S2- is bonded in a 4-coordinate geometry to one Cs1+ and four Mo+2.40+ atoms. In the fourth S2- site, S2- is bonded in a 7-coordinate geometry to one Cs1+ and three equivalent Mo+2.40+ atoms. In the fifth S2- site, S2- is bonded in a 4-coordinate geometry to one Cs1+ and three equivalent Mo+2.40+ atoms.